Fracture Mechanics of Composites with Residual Thermal Stresses


 Frank Young
 1 years ago
 Views:
Transcription
1 J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate for crack growth in an arbitrary composite in the presence of residual stresses is considered. First, a general expression is given for arbitrary, mixed traction and displacement boundary conditions. This general result is then applied to a series of specific problems including statistically homogeneous composites under traction or displacement boundary conditions, delamination of double cantilever beam specimens, and microcracking in the transverse plies of laminates. In many examples, the energy release rate in the presence of residual stresses can be reduced to finding the effect of damage on the effective mechanical properties of the composite. Because these effective properties can be evaluated by isothermal stress analysis, the effect of residual stresses on the energy release rate can be evaluated without recourse to any thermal elasticity stress analyses. Introduction When a composite comprised of materials having disparate thermal expansion coefficients is subjected to a uniform change in temperature, it will develop residual thermal stresses. If that composite develops cracks, either as a result of the residual thermal stresses or of some subsequently applied mechanical tractions, the residual and mechanical stresses will change to accommodate the fracture surfaces. One effect of the redistribution of residual thermal stresses is a change in the effective thermal expansion coefficient of the composite Hashin, 988. Additionally, the redistribution of residual and mechanical stresses releases strain energy that can drive crack propagation the energy release rate for crack growth. The goal of this paper is to evaluate the effect of residual thermal stresses on the energy release rate for crack growth in composites. The redistribution of residual and mechanical stresses caused by cracks can be viewed as similar elasticity problems but with different boundary conditions. Because of their similarity, it is often possible to explicitly account for the effect of residual thermal stresses without doing a thermal elasticity analysis of the composite. Some general energy release rate expressions including residual thermal stresses are derived in the first section of this paper. The general results are for an arbitrary composite under arbitrary, mixed traction and displacement boundary conditions. Next, the general expressions are applied to statistically homogeneous composites, double cantilever beam delamination specimens, and microcracked laminates. The simplest possible energy release rate expressions are derived. In some examples, the energy release depends on knowledge of both the mechanical and residual stress states, but, in some important practical examples, the energy release rate can be expressed in terms of the effect of cracks on the effective composite mechanical properties. These effective mechanical properties can be derived using elasticity analyses that ignore residual stresses. General Theory Consider an arbitrary, multiphase composite subjected a uniform temperature change of T = T and to any mixed traction and displacement boundary conditions. Let the surface be S = S T S u, where S T is that part of the surface subjected to traction boundary conditions: T = T 0 = σ 0ˆn where σ 0 is the surface applied stress note: all tensors are written in boldface and ˆn is a unit normal to the surface. S u is that part of the surface subjected to displacement boundary conditions: u = u 0 = ε 0 x 804 / ol. 64, DECEMBER 997 Transactions of the ASME
2 where ε 0 is the surface strain and x is a position vector on the surface. T 0 and u 0 are the boundary conditions; in general they may depend on position. Note also that tractions and displacements may be applied over the same portions of the surface provided they are applied along different coordinates. For example, one section of the surface may have traction in the x direction but fixed displacement in the y direction. Similar to Rosen and Hashin 970, the full thermal elasticity problem can be treated as a superposition of two problems. First, let σ m and ε m, with tractions T m and displacements u m, be the solution to the isothermal T = 0 elasticity problem: σ mˆn = T 0 on S T 3 u m = u 0 on S u 4 σ m = Cε m and ε m = Sσ m 5 where C and S are the stiffness and compliance tensors. In a composite, C and S will depend on position. As the solution to an elasticity problem, σ m satisfies equilibrium and ε m satisfies compatibility. Second, let σ r and ε r, with tractions T r and displacements u r, be the solution to the thermal elasticity problem: σ rˆn = 0 on S T 6 u r = 0 on S u 7 σ r = Cε r αt and ε r = Sσ r + αt 8 where α is the positiondependent thermal expansion tensor, σ r satisfies equilibrium, and ε r satisfies compatibility. Note that T r may be nonzero on S u and u r may be nonzero on S T. A superposition of the above two solutions, σ = σ m + σ r and ε = ε m + ε r, solves the complete thermal elasticity problem σ ˆn = T 0 on S T 9 u = u 0 on S u 0 σ = Cε αt and ε = Sσ + αt σ m and ε m are the mechanical stresses and strains while σ r and ε r are the residual thermal stresses and strains. The internal energy is the volume integral of stress dotted into strain relative to the freeexpansion strains. This energy can be expressed in terms of mechanical and residual stresses: U = σ ε αt d = σ m Sσ m d + σ m Sσ r d + σ r Sσ r d Assuming tractionfree crack surfaces and using the divergence theorem, the mechanical stress term in Eq. may be written in terms of mechanical surface tractions, T m, and displacements, u m, as σ m Sσ m d = T 0 u m ds + T m u 0 ds 3 S T S u T 0 u r ds 4 For the cross term in Eq., the displacements caused by the residual thermal stresses can be considered as virtual displacements to the mechanical strains or δ u = u r. They correctly have u r = 0 on S u. By virtual work σ m ε r d = S T But also, ε r = Sσ r + αt, giving σ m Sσ r d = T 0 u r ds σ m αt d 5 S T Analogously, the residual tractions, T r, can be considered as virtual forces on the mechanical stresses; σ r obeys equilibrium and T r = 0 on S T. Thus, again by virtual work ε m σ r d = σ m Sσ r d = T r u 0 ds 6 S u Journal of Applied Mechanics ol. 64, DECEMBER 997 / 805
3 Finally, for the pure residual stress term in Eq. : σ r Sσ r d = σ r ε r σ r αt d = S T r u r ds σ r αt d 7 But, over the entire surface, either T r = 0 or u r = 0, giving σ r Sσ r d = σ r αt d 8 Combining Eqs. 3, 5, 6, and 8 gives U = T 0 u m ds + T m u 0 ds + T r u 0 ds σ r αt d 9 S T S u S u σ m αt = T 0 u r ds T r u 0 ds 0 S u S T For fracture mechanics analysis we need to evaluate the energy release rate defined as G = dw du where W is external work and A is fracture area. The external work is caused by the action of the mechanical tractions on S T applied over the total displacements. Thus dw = d T 0 u m + u r ds Combining this result with Eqs. 9 and 0 gives G = G mech + T S T d σm α + d σr α where G mech is the mechanical energy release rate or the energy release when T = 0: G mech = d T 0 u m ds T m u 0 ds S T and angle brackets indicates a volumeaveraged quantity: fx, y, z = fx, y, zd 5 Note that the full, thermodynamic internal energy in thermal elasticity includes heat capacity terms. The energy associated with residual stresses that exist under zero traction or zero displacement, can be viewed as contributing to the effective constant pressure or constant volume heat capacity of the composite Rosen and Hashin, 970. Here the residual stress energy contributes to the total energy release rate for crack growth. The heat capacity terms associated with individual phases, however, can be ignored when calculating energy release rates because they drop out when the derivative with respect to crack area is evaluated. The result in Eq. 3 includes nothing specific about composites. The result for a composite with n phases is G = G mech + T v i α i S u dσim + dσir where superscript i means a property of phase i, v i is the volume fraction of phase i, and the over bar indicates a phaseaveraged quantity integrated over the volume of phase i, i : σ im = σ m d 7 v i i 806 / ol. 64, DECEMBER 997 Transactions of the ASME 3 4 6
4 In deriving Eq. 6, it was assumed that the component thermal expansion tensors in each phase are independent of position within that phase. This situation always holds for composites with isotropic phases. For composites with anisotropic phases at variable orientations, each orientation must be considered as a separate phase for analysis by Eq. 6. When anisotropic phases are aligned, such as in unidirectional, carbonfiber reinforced composites, the anisotropic phase can be considered as a single phase. Although the general result in Eq. 6 depends on both mechanical and thermal stresses, in some important special cases, the energy release rate can be expressed solely in terms of mechanical properties and stresses. For example, in many fracture situations, cracks will propagate such that failure is by pure mode I fracture or pure opening mode fracture. For example, it has been suggested that regardless of external loading conditions that delamination always proceeds by mode I fracture Charalambides et al., 99. Under pure mode I crack growth, energy release rate is related to mode I stress intensity factor by G I K I 8 In linear thermal elasticity, K I must be linearly related to applied load and temperature change. If we thus consider uniformly scaling all applied tractions and displacements to be where P is a scalar multiplier, stress intensity must have the form T app = P T 0 and u app = P u 0 9 K I = c P + c T 30 where c and c are some constants that depend on material properties and geometry of the crack. The energy release rate must therefore have the form Comparing Eq. 3 to Eq. 6 we can prove that G I c P + c T 3 T Substitution back into Eq. 6 gives v iα i dσim = v iα i dσir G mech v iα i dσim G I = + T G mech v iα i dσim G mech 3 33 Remarkably, the energy release rate including residual thermal stresses depends only on the results from a mechanical stress analysis. Thus, the effect of residual stresses can be determined without any need for solving a thermal elasticity problem. Although this result was derived for pure mode I crack growth, analogous expressions hold for pure mode II or III crack growth. Examples Uniform Traction, Statistically Isotropic Composite A useful model for evaluating effective properties of composite materials is to consider a statistically homogeneous composite Hashin, 963; 969. Such composites are analyzed by averaging over a representative volume element; this element must be chosen large enough to have all averaged results representative of the averaged results for entire composite Hashin, 963; 969. Here we also consider the representative volume element to have cracks that are representative of the entire composite. Such a representative volume element is then subjected to a uniform traction or a traction that arises from a surface stress, σ 0, that is independent Journal of Applied Mechanics ol. 64, DECEMBER 997 / 807
5 of position. By the average strain theorem Hill, 963; Hashin 963; 969, the only remaining integral in G mech reduces to T 0 u m ds = S σ0 ε m D m = σ0 S σ 0 34 where S is the effective compliance tensor of the composite Hashin, 963; 969. The tensor D m is related to the crack opening mechanical displacements and is defined by Dij m = u m j n i + u m i n j ds i, j = x, y, or z 35 S c where S c is total crack surface area. The effective composite compliance is defined in terms of the apparent average strain which is the bulk average strain reduced by the crackopening tensor Aboudi, 994; thus S σ 0 = ε m D m 36 Substituting Eq. 34 into Eq. 6 the energy release rate becomes G = σ 0 ds σ0 + T v i α i dσim For pure mode I or II, or III crack growth the energy release rate becomes G I G mech = + T v iα i dσim σ 0 ds σ0 ] + dσir Finally, for a two phase composite a composite with two isotropic phases or two aligned anisotropic phases we have S v dσ m dσ v m + v dσ m + S v dσ m = 0 39 = d εm = ds σ0 + ddm For pure mode fracture we can derive ] σ G I = 0 + T α α S S ds σ0 + T α α S S ddm 4 σ 0 ds σ0 The energy release rate depends only on the effective compliance tensor and the mechanicallyinduced crackopening displacement tensor. Note the D m only affects the energy release rate when there are residual thermal stresses; in the absence of residual stresses, G I depends only on S. Uniform Displacement, Statistically Isotropic Composite For uniform displacement u 0 = ε 0 x where ε 0 is independent of position applied to a statistically homogeneous composite, use of the average stress theorem leads to G mech = d σ m 40 ε0 = ε0 dc ε0 4 where C is the effective stiffness tensor of the composite. For a better analogy with the uniform traction results, some terms can be reexpressed as: α i σ im = M i ε im 43 α i σ ir = M i ε ir + α i M i T / ol. 64, DECEMBER 997 Transactions of the ASME
6 P u y x u P Fig. A double cantilever beam specimen using unidirectional composites. The fiber direction indicated by the internal lines is parallel to the delamination crack growth. The specimen is point loaded by loads of P. The total deflection between the loading points is u. where M = Cα is the stresstemperature tensor. Incorporating these results into the Eq. 6 and ignoring the constant term α i M i T, which drops out upon differentiation, the energy release rate is ] G = ε 0 dc ε0 + T v i M i dεim + dεir 45 This result is identical to the uniform traction results see Eq. 37 except for a sign change and physical meanings of all symbols. The sign change is required because G is positive and, in general, C decreases with crack growth. By an explicit analogy to the results for uniform traction, the energy release rate for pure mode crack growth becomes Delamination G I G mech = + T v im i dεim ε 0 dc ε0 Figure shows a double cantilever beam specimen made from a unidirectional composite. The fibers run parallel to the x direction. This problem differs from the previous sections in two respects. First, the specimen is not statistically homogeneous because there is only one macroscopic delamination crack. Second, although there is only traction loading, the tractions are not uniform i.e., they depend on position. The tractions can be written as T 0 = P δ x x upper δ x x lower ] 47 where δ x is the Dirac delta function and x upper and x lower are the locations of the upper and lower load points. Substitution into Eqs. 4 and 33 because the crack growth is pure mode I gives v iα i dσim G I = P dc m + T P dc m where C m = u m /P is the mechanical loadpoint compliance. The leading term is G mech or the energy release rate in the absence of residual stresses Proceeding for a twophase unidirectional composite fibers as phase and matrix as phase with aligned transversely isotropic phases, we can write v i α i dσim = v σ xx m α A + σ yy m + σ m zz ] α T + v σ xx m α A + σ yy m + σ m zz ] α T Journal of Applied Mechanics ol. 64, DECEMBER 997 /
7 σ 0 σ 0 x 90 Plies t z s n B σ 0 σ 0 Fig. An edge view of a microcracked laminate. The microcracks occur in the central 90 plies; they are located at the top and bottom of the 90 plies are are separated by a distance s. Each ply has thickness t i ; the total symmetric laminate thickness is B. Now, doublecantilever beams specimens without residual stresses can be well analyzed using beam analyses Hashemi et al., 990. Within the assumptions of a beam analysis σ yy im and σ zz im are identically zero while σ xx im will net to zero by virtue of a balance between tension and compression stresses within the beam. The energy release rate for delamination becomes simply G = P dc m 50 In other words, within the assumptions of beam analyses, residual stresses have no effect on delamination. Residual stresses are present in both the fiber and the matrix, but they release no energy as the delamination propagates. Microcracked Laminate Figure shows an edge view of a symmetric, nply laminate under a uniaxial load of σ 0 in the x direction in which the central 90 ply group has throughthewidth cracks separated by a distance s. This geometry is appropriate for analysis of a microcracked laminate with periodic microcracks in the 90 plies having a density D = /s Nairn and Hu, 994. This problem differs from previous examples in three respects. First, the tractions are nonuniform: σ 0 is applied to the uncracked plies, but there is zero traction on the cracked 90 plies. Second, there are more then two phases. Although the plies themselves are composites, here each ply is treated as a homogeneous, anisotropic material. The general laminate, which may have plies at many orientations or may even be a hybrid laminate, is thus a multiphase composite. Third, we incorporate information about the laminated structure of the composite into the analysis. The key structural information we use is that the x and y direction strains of all uncracked plies are equal and that σ zz im plies. From Eq. 3, we can immediately write G = = σ ir zz = 0 in all d σ 0 + T σ m α + σ r α 5 80 / ol. 64, DECEMBER 997 Transactions of the ASME
8 where E xx is the effective laminate modulus in the x direction. The first term is the energy release rate in the absence of residual stresses. Furthermore, by Eq. 0 we can write σ m αt = σ 0 ε r xx u = σ 0 α xxt 5 where αxx is the effective laminate thermal expansion coefficient in the x direction and ε r xx u is the volume averaged residual strain in the uncracked plies only. This term appears because the tractions are applied only to the uncracked plies. Equation 5 is similar to Levin s analysis for thermal expansion coefficient of a composite Levin, 967; Rosen and Hashin, 970 except that it is applied here under conditions of nonuniform traction. The energy release rate will be analyzed first using a plane stress analysis in which σ yy im all plies. From Eq. 5: σ 0 α xx = = σ ir yy = 0 in v i σ xx im α xx i 53 where v i = t i /B is the total volume fraction of ply i including both sides of the symmetric laminate. By force balance and isostrain in the uncracked plies v i σ xx im = σ 0 and σ xx im = Ei xxσ 0 for i 54 Using these results, the effective xdirection thermal expansion coefficient can be expressed as αxx = α xx i v α xx E xx u E xx 55 where α xx = α xx α u xx, E xx u i= = v ie xx i, and α u i= xx = v iα i v n i= v ie xx i xxe xx i E xx u and α xx u are the ruleofmixtures xdirection modulus and thermal expansion coefficient of the uncracked plies. The residual strain energy term is σ r αt = By force balance of residual stresses and isostrain in the uncracked plies v i σ xx ir = o and σ xx ir Using these results, the residual strain energy term is 56 v i σ ir xx α i xxt 57 = E xx i α xx α i xx T for i 58 σ r αt = constant α xx v T α xx E u xx 59 The constant term is not evaluated because it drops out when finding the energy release rate. Substituting Eqs. 5, 55, and 59 into Eq. 5 gives G = d σ 0 α xx E xx u v T E xx 60 The energy release rate in the presence of residual thermal stresses depends only on one effective property E xx; that property can be evaluated by an isothermal stress analysis. If we imagine formation of a complete new microcrack midway between two existing microcracks, we have = BW s = BW D and = t W = v BW 6 Journal of Applied Mechanics ol. 64, DECEMBER 997 / 8
9 The integrated energy release rate for formation of a complete microcrack is G = σ 0 α xx E xx u v T v D 6 where /E xx is the change in the effective xdirection modulus caused by the new microcrack. An energy release expression mathematically identical to Eq. 6 is given in a different form in Nairn et al. 993 and Nairn and Hu 994 and in the identical form in Nairn 995. In Nairn et al. 993, Nairn and Hu 994, and Nairn 995, however, the energy release rate was the specific result of a thermal elasticity analysis. Here the energy release rate is derived as a general result. The accuracy of finding G is only limited to the accuracy in finding E xx. In Nairn 995, variational mechanics was used to bound E xx and an average of those bounds gave a virtually exact solution for G. A better connection with laminated plate theory can be derived by considering a generalized planestrain analysis of a cracked laminate instead of the previous plane stress analysis. In the generalized planestrain analysis, it is assumed that the ydirection strain in all plies is ν xyσ 0 /E xx where ν xy is the effective xy Poisson s ratio of the cracked laminate. The resulting new analysis will correct the plane stress analysis to account for differential Poisson s ratios between the plies. The corrections are generally small, but can be accomplished in a straightforward analysis. Equations 5 and 5 are unchanged in the generalized planestrain analysis. Starting from Eq. 5: σ 0 α xx = v i σ xx im xx + v i σ yy im α yy i α i 63 By force balance and isostrain in the uncracked plies v i σ im xx = σ 0 and σ im xx = Q i ν xyq i σ0 σ yy im = Q i ν xyq i σ0 E xx v i σ im yy = 0 64 for i 65 for i 66 where Q i kj k, j =,, 6 are the suitablyrotated elements of the inplane stiffness matrix for ply i Tsai, 987. Using these results, the effective xdirection thermal expansion coefficient becomes α xx = α xx + E xx i= ν xy E xx ] v i α xx i α xx Q i + α yy i α yy Q i i= ] v i α xx i α xx Q i + α yy i α yy Q i 67 Now consider the laminate created by removing the cracked plies and joining the remaining plies; call it the uncracked laminate. By laminated plate analysis of the symmetric uncracked laminate Tsai, 987, it can be shown that i= i= v i Q i i= v i α xxq i i + αi yy Q i v i α xxq i i + αi yy Q i kj = Au kj = B = B B A u αu xx + A u αu yy A u αu xx + A u αu yy / ol. 64, DECEMBER 997 Transactions of the ASME
10 where A u kj are the elements of the laminated plate theory A] matrix for the uncracked laminate and α xx u and α yy u are the thermal expansion coefficients for the uncracked laminate defined by: α u xx = B α u yy = B a u a u i= i= v i α xxq i i + αi yy Q i + a u v i α xxq i i + αi yy Q i + a u i= i= ] v i α xxq i i + αi yy Q i 7 ] v i α xxq i i + αi yy Q i 7 Here a u kj are elements of the laminated plate theory a] matrix which is the inverse of the A] matrix. Using these results, the effective xdirection thermal expansion coefficient can be expressed as αxx = α xx v + ν xy v 73 where = = B v B v A u A u α xx α xx u α xx α xx u ] + A u α yy α yy u ] + A u α yy α yy u Note that A u kj /B v are the elements of the normalized, x y plane stiffness matrix for the uncracked laminate Tsai, 987. By a similar analysis but with σ 0 applied in the y direction, the effective ydirection thermal expansion coefficient can be expressed as αyy = α yy v Eyy + ν xy v 76 The residual strain energy term is σ r αt = v i σ ir xx α i xxt + v i σ yy ir α yy i T 77 By force balance of residual stresses and isostrain in the uncracked plies σ ir xx σ ir yy v i σ ir xx = 0 and = Q i αxx α xx i = Q i α xx α i xx T + Q i T + Q i Using these results, the residual strain energy term is v i σ ir yy = 0 78 α yy α i yy α yy α i yy T for i 79 T for i 80 σ r αt = constant α xx v T α yy v T 8 The constant term is not evaluated because it drops out when finding the energy release rate. Substituting Eqs. 5, 73, 76, and 8 into Eq. 5 gives G = d d ν xy σ 0 v T + v T σ 0 v T ] + v T d 8 E yy Journal of Applied Mechanics ol. 64, DECEMBER 997 / 83
11 The energy release rate depends only on, Eyy, and νxy, all of which can be evaluated by an isothermal stress analysis. Equation 8 is exact for any damage mode in a microcracked laminate. If the damage is mode I propagation of a new microcrack between the existing microcracks, we can use Eq. 3 to derive an exact relation between laminate effective properties: d d ν xy E xx = d d E yy ν 83 xy Interestingly, an analysis of fracture in the presence of residual thermal stresses has lead to a relation between effective mechanical properties. Using Eq. 83 the mode I microcracking energy release is G I = σ 0 v T d d E xx E xx + v T d ν ] xy 84 The mode I energy release rate depends only on and νxy. McCartney 994 derived results that appear equivalent to Eqs. 8 and 83. McCartney s results, however, were a specific result of an approximate generalized, planestrain, thermal elasticity analysis of a microcracked laminate. The results here were derived by a very different path and are exact provided exact results for, νxy, and Eyy are known. The previous results were for uniaxial loading. It is trivial to extend the analysis to generalized inplane loading of the microcracked laminate. The energy release rate becomes G = d E ν xy xx E 0 xx Note: / is a σeff ν xy Eyy 0 σ eff correction vs published paper G xy where G xy is the effective inplane shear modulus and σ eff is the effective inplane applied stressed defined by σ eff = σ x0 v T, σ y0 v T, τ xy0 86 Here σ x0, σ y0, and τ xy0 are the applied inplane stresses. Discussion In many examples considered, the energy release rate for crack growth, G, was reduced to an expression that depends only on the effective compliance S or stiffness C tensors and the phase average mechanical stresses. Because these terms can be evaluated by isothermal elasticity methods Hashin 963; 969, it is often possible to include the effect of residual thermal stresses on the energy release rate without ever evaluating the thermal stresses. In other words, no thermal elasticity analysis of the composite is required. This result, however, does not imply that the effect of residual thermal stresses is a trivial extension of isothermal fracture mechanics analysis. For example, the isothermal energy release rate for microcracking of a laminate depends only on the. In contrast, the energy release rate in the presence of residual stresses depends on, νxy, and Eyy. Thus, in general, the fracture mechanics analysis of a composite with residual thermal stresses will require more isothermal elasticity analysis of composite properties than the corresponding isothermal fracture mechanics analysis. The discussion here was confined to residual thermal stresses, but identical results could be derived for other types of residual stresses. For example, fiberreinforced, polymermatrix composites can develop residual stresses due to differential moisture absorption between the fibers and the matrix Tsai, 987. The results for moistureinduced residual stresses can be generated from the results given here by replacing α by the moisture expansion tensor and T by the moisture concentration. Residual stresses induced by nonuniform 84 / ol. 64, DECEMBER 997 Transactions of the ASME
12 temperature T a function of position are more complicated. The general theory derived here up to Eq. 3 still applies when there is nonuniform T. Many subsequent simplifications, however, only hold for uniform T. The energy release rate in the presence of residual stresses depends on derivatives of mechanical terms like ds, dc, and dσ im 87 Many damage mechanics models have been developed that give effective properties as a function damage. The results in this paper could easily be incorporated into such models to simultaneously give the energy release rate for damage growth. An important observation, however, is that the ability of a damage analysis to predict effective properties is necessary but not sufficient justification for use of that analysis to calculate energy release rate. The problem is that calculating derivatives of effective properties is a harder problem than calculating the average property itself. Analyses that are accurate to within a few percent for effective properties may be grossly in error when calculating the derivative. Thus any damage mechanics analysis that seeks to calculate energy release rate must be verified to have accurate derivatives of the required terms. Experimentally this verification can be done by comparing fracture experiments to fracture mechanics predictions. In contrast, experimental verification based on effective property predictions, such as modulus reductions, are inadequate tests of energy release rate models. Acknowledgments This work was supported, in part, by a grant from the Mechanics of Materials program at NSF CMS , and, in part, under McDonnell Douglas contract NAMP References Aboudi, J., 994, Interfacial Damage, Damage Mechanics of Composite Materials, ed., Ramesh Talreja, Elsevier, Amsterdam, pp Charalambides, M., A. J. Kinloch, Y. Wang, and J. G. Williams, 99, On the Analysis of MixedMode Failure, Int. J. Fract., ol. 54, pp Hashemi, S., Kinloch, A. J., and Williams, J. G., 990, The Analysis of Interlaminar Fracture in Uniaxial Fibre Reinforced Polymer Composites, Proc. R. Soc. Lond., ol. A347, pp Hashin, Z., 963, Theory of Mechanical Behavior of Heterogeneous Media, Applied Mechanics Reviews, ol. 7, pp. 9. Hashin, Z., 969, Theory of Composite Materials, Mechanics of Composite Materials, Pergamon Press, pp Hashin, Z., 988, Thermal Expansion Coefficients of Cracked Laminates, Comp. Sci. & Tech., ol. 3, pp Hill, R., 963, Elastic Properties of Reinforced Solids: Some Theoretical Principles, J. Mech. Phys. Solids, ol., pp Levin,. M., 967, On the Coefficients of Thermal Expansion in Heterogeneous Materials, Mechanics of Solids, ol., pp McCartney, L. N., 994, The Prediction of NonUniform Cracking in Biaxially Loaded CrossPly Laminates, National Physical Laboratory, Teddington, United Kingdom, Report DMMA 4. Nairn, J. A., Hu, S., and Bark, J. S., 993, A Critical Evaluation of Theories for Predicting Microcracking in Composite Laminates, J. Mat. Sci., ol. 8, pp Nairn, J. A., and Hu, S., 994, Micromechanics of Damage: A Case Study of Matrix Microcracking, Damage Mechanics of Composite Materials, ed., Ramesh Talreja, Elsevier, Amsterdam, pp Nairn, J. A., 995, Some New ariational Mechanics Results on Composite Microcracking, Proc. 0 th Int l Conf. on Comp. Mat., ol. I, pp Rosen, B. W., and Hashin, Z., 970, Effective Thermal Expansion Coefficients and Specific Heats of Composite Materials, Int. J. Engng. Sci., ol. 8, pp Tsai, T. W., 987, Composites Design, Think Composites, Dayton, Ohio. Journal of Applied Mechanics ol. 64, DECEMBER 997 / 85
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationThe Initiation and Growth of Delaminations Induced by Matrix Microcracks in Laminated Composites
International Journal of Fracture, 57, 1 4 199. The Initiation and Growth of Delaminations Induced by Matri Microcracks in aminated Composites J. A. NAIRN and S. HU Department of Materials Science and
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationOn the calculation of energy release rates for cracked laminates with residual stresses
International Journal of Fracture, 39, 67 93 006) On the calculation of energy release rates for cracked laminates with residual stresses J. A. NAIRN Wood Science and Engineering, Oregon State University,
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationCross Laminated Timber Properties Including Effects of NonGlued Edges and Additional Cracks
European Journal of Wood and Wood Products Volume 75, Issue 6, pp 973 983 7) Cross Laminated Timber Properties Including Effects of NonGlued Edges and Additional Cracks John A. Nairn Received: 9 January
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationNumerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board
Numerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board John A. Nairn (Professor) and Edward Le (PhD Student) Wood Science & Engineering,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationFracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments
Engineering Fracture Mechanics ) 4 Author prepared preprint Fracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments SungRyong Kim a, John A. airn
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationIntroduction to Finite Element Method
Introduction to Finite Element Method Dr. Rakesh K Kapania Aerospace and Ocean Engineering Department Virginia Polytechnic Institute and State University, Blacksburg, VA AOE 524, Vehicle Structures Summer,
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationChapter 3 LAMINATED MODEL DERIVATION
17 Chapter 3 LAMINATED MODEL DERIVATION 3.1 Fundamental Poisson Equation The simplest version of the frictionless laminated model was originally introduced in 1961 by Salamon, and more recently explored
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationThis Technical Note describes how the program checks column capacity or designs reinforced concrete columns when the ACI code is selected.
COMPUTERS AND STRUCTURES, INC., BERKELEY, CALIFORNIA DECEMBER 2001 CONCRETE FRAME DESIGN ACI31899 Technical Note This Technical Note describes how the program checks column capacity or designs reinforced
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationContemporary Research in Engineering Science
Bazant, Z.P., and Prat, P.C. (1995). 'Elastic material with systems of growing or closing cracks: Tangential Stiffness.' in Contemporary Research in Engineering Science (Proc., Eringen Medal Symp. honoring
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationVirtual distortions applied to structural modelling and sensitivity analysis. Damage identification testing example
AMAS Workshop on Smart Materials and Structures SMART 03 (pp.313 324) Jadwisin, September 25, 2003 Virtual distortions applied to structural modelling and sensitivity analysis. Damage identification testing
More informationThe concept of Representative Volume for elastic, hardening and softening materials
The concept of Representative Volume for elastic, hardening and softening materials Inna M. Gitman Harm Askes Lambertus J. Sluys Oriol Lloberas Valls i.gitman@citg.tudelft.nl Abstract The concept of the
More information2 Introduction to mechanics
21 Motivation Thermodynamic bodies are being characterized by two competing opposite phenomena, energy and entropy which some researchers in thermodynamics would classify as cause and chance or determinancy
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationStrainBased Design Model for FRPConfined Concrete Columns
SP230 57 StrainBased Design Model for FRPConfined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strainbased confinement model is developed herein for circular concrete columns
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationMalaysia Phone: ; Fax:
International Conference on Mechanical Engineering Research (ICMER013), 13 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia
More information